monitoring of the process of flash-butt of the process of flash-butt welding ... the monitoring of...
Post on 23-May-2018
Embed Size (px)
(Recebido em 02/04/2012; Texto final em 18/09/2012).
Monitoring of the Process of Flash-Butt Welding
(Monitoramento do processo de soldagem de topo por faiscamento)
Yevgenia Chvertko, Mykola Shevchenko, Andriy PirumovNational Technical University of Ukraine Kyiv Polytechnic Institute, Kyiv, Ukraine, email@example.com, firstname.lastname@example.org,
Statistical methods of analysis are currently widely used to develop control and monitoring systems for different welding processes. These methods allow to obtain information about the process including effect of all factors on its results, which is often difficult to evaluate due to the complexity of the process. The authors made efforts to apply these methods to develop the system for monitoring the parameters of flash-butt welding in real-time mode. The paper gives brief information about the features of flash-butt welding of reinforcement bars and some basic limitation of this process application. The main reasons of formation of defects in welded joints are given as well as analysis of possibility of application of monitoring systems for their determination. The on-line monitoring system based on neural networks was developed for evaluation of process deviations. This system is believed to be adequate for determination of process violations resulting in disturbances of welding parameter and can be used for prediction of possible defects in the welded joints.
Key-words: Flash-butt welding, Defects in joints, Neural networks, Quality monitoring
Resumo: Anlises estatsticas so normalmente utilizadas para desenvolver sistemas de controle e monitoramento de diferentes processos de soldagem. Estes mtodos permitem obter informao sobre o processo, incluindo o efeito de todos os fatores sobre o resultado, os quais so difceis de avaliar devido a complexidade do processo. Os autores do presente trabalho tentaram aplicar estes mtodos para desenvolver um sistema de monitorao dos parmetros da soldagem de topo por faiscamento em tempo real. O artigo d uma ideia resumida sobre as caractersticas do processo de soldagem por faiscamento de vergalhes, assim como some limitaes bsicas da aplicao do processo. As razes principais para formao de defeitos na junta soldada so apresentadas, assim como a anlise da possibilidade da aplicao de um sistema de monitorao para suas determinaes. Um sistema em tempo real baseado em redes neurais para avaliar as variaes do processo foi desenvolvido e apresentado. Este sistema considerado adequado para determinar as no conformidades do processo, e pode ser usado para predizer possveis defeitos na junta soldada.
Palavras-chave: Soldagem de topo por faiscamento, Defeitos, Redes neurais, Qualidade monitorao
At the present time the welding process is considered to consist of three operations : the welding procedure specification, welding itself and after-welding check. All the operations mentioned require application of different methods of control and monitring. During the welding procedure specification the preparation of parts to be welded is checked as well as preliminary cleaning, heat-treatment, welding consumables and process parameters. The process of welding is followed by selective or continuous monitoring. The after-welding check includes determination of quality parameters, analysis of posiible reasons of formation of defects and as a result updating
the welding procedure and parameters (if needed).Evaluation methods based on statistical analysis and statistical quality control technologies are often used in welding, especially for after-welding check. Such quality control methods allow to improve the system and organization of control . Statistical methods do not replace the other methods of control, but they significantly improve their effectiveness, adequacy and economical characteristics.Every welding process consists of two components: one is determined by the pre-set welding parameters and resources used, the second one appears due to different physical processes occuring during welding (they depend on the process nature, conditions in which welfing is run and all the internal and external disturbances). It is almost impossible to determine all such side processes, meaning the exact influence of each factor on the quality of the welded joint cannot be definitely described. Statistical analysis allows to evaluate the process in whole and in such way to take into consideration the effect of all factors irrelatively to their nature.
Soldag. Insp. So Paulo, Vol. 18, N. 01, p.031-038, Jan/Mar 2013
Yevgenia Chvertko, Mykola Shevchenko, Andriy Pirumov3
Some prospective studies are devoted to evaluation of quality characteristics by energetic parameters of the welding process. This approach is believed to be the most applicable in case of mass production because these parameters are easy to measure without additional equipment and human resources. The analysis results are used mainly for three purposes: to predict the quality characteristics of the welded joint (possible defects, mechanical properties and geometry), to define the disturbances occuring during the process and for continuous process monitoring. Such analysis if often performed by means of intellectual systems which allow to remove the human from the procedure of control and thus to reduce the subjectivity of its results and the process cost. At the present time such monitoring systems are used for arc welding and resistance spot welding [3, 4].The objective of this work was to investigate the posibility of application of methods of statistical analysis as well as artificial intelligence systems for monitoring of flash-butt welding process of concrete reinforcement bars. The monitoring will be based on the analysis of energetic parameters of the welding process.
2. The monitoring of the process of flash-butt welding of reinforcement bars
2.1. Technology of flash-butt welding of reinforcement bars in construction of structures of monolithic reinforced concrete
In construction and repair of reinforced concrete structures the different methods of arc welding of concrete reinforcement are used. The manual and semi-automatic electric arc welding, bath-arc welding and others have found the widest spreading. It should be noted that at plants and industrial groups of as-assembled reinforced concrete a flash-butt welding with a continuous flashing is widely used, except the above-mentioned methods. Now, it is one of main methods of producing the butt joints of concrete reinforcement under the shop conditions.The flash-butt welding is characterized by a high stable quality of welded joints, almost equal in strength to the parent metal that makes it possible to increase greatly the reliability and
service life of reinforced concrete structures and to provide the high productivity. The process of welding is performed in the automatic conditions, combines the assembly and welding operations in a single cycle, does not require application of auxiliary consumables (electrodes, welding wire, fluxes, gases, etc.). Moreover, special requirements to the welders qualification are not specified.At the present time, special technologies and equipment are being developed to make it possible to use this welding method in on-site and semi-stationary conditions . The method application is also partially limited by existing quality control procedures . This rises the problem of development of technologies of non-destructive real-time monitoring.As a rule, the concrete reinforcement, bars of up to 22 mm are joined by the flash-butt welding with a continuous flashing, and the large-diameter bars are joined by using a flashing with a preliminary resistance preheating. The latter is characterized by a wide instable HAZ. The flash-butt welding with a pulsed flashing allows joining all the assortment of reinforced bars and has advantages over the above-mentioned methods. Mechanical characteristics of these steels in hot-rolled state are given in Table 1, and chemical composition is given in Table 2.The carried out technological investigations of welding the hot-rolled reinforcement bars made it possible to establish the values of main parameters of welding conditions: adjusting length Ladj, tolerances for flashing Lflash and upsetting Lupset, open-circuit secondary voltage U2o.-c rates of flashing vflash, and upsetting vupset, time of welding and time of upsetting with current tupsetI [6, 8].The increased sensitivity to heating of heat-hardened reinforcement bars specifies the additional requirements to thermal cycles of heating in welding and increases greatly the requirements to the selection of its heating conditions during welding. Using the welding parameters with smaller tolerances for flashing usually causes the brittle fracture because of an intensive heat dissipation into welding machine electrodes being cooled. The recent technological investigations resulted in development of welding cycles for heat-hardened reinforcement bars which allow to produce welded joints almost equal in strength to the parent metal .
Table 1. Mechanical characteristics of bar reinforcing steelsSteel grade
t, MPa , %
35GS 370 500 610 670 18 30
25G2S 380 400 590 620 23 31
St3Gsp 235 370 - 490 25
Table 2. Chemical composition of bar reinforcing steels, wt.%Steel grade
C Mn Si Cr Ni S P Cu
35GS 0.20 0.29 1.20 1.60 0.60 0.90
33Soldag. Insp. So Paulo, Vol. 18, N. 01, p.031-038, Jan/Mar 2013
Monitoring of the Process of Flash-Butt Welding
2.2. Analysis of possibility of application of the system of monitoring for determination of defects
In general the defects in the welded joints of reinforcement bars appear as a result of th